Diamond-like carbon (DLC) exists in seven different forms of amorphous carbon materials that display some of the unique properties of diamond. They are usually applied as coatings to other materials that could benefit from some of those properties. All seven contain significant amounts of sp3 hybridized carbon atoms. The reason that there are different types is that even diamond can be found in two crystalline polytypes. The usual one has its carbon atoms arranged in a cubic lattice, while the very rare one (lonsdaleite) has a hexagonal lattice. By mixing these polytypes in various ways at the nanoscale level of structure, DLC coatings can be made that at the same time are amorphous, flexible, and yet purely sp3 bonded "diamond". The hardest, strongest, and slickest is such a mixture, known as tetrahedral amorphous carbon, or ta-C. For example, a coating of only 2 μm thickness of ta-C increases the resistance of common (i.e. type 304) stainless steel against abrasive wear; changing its lifetime in such service from one week to 85 years. Such ta-C can be considered to be the "pure" form of DLC, since it consists only of sp3 bonded carbon atoms. Fillers such as hydrogen, graphitic sp2 carbon, and metals are used in the other 6 forms to reduce production expenses or to impart other desirable properties. The various forms of DLC can be applied to almost any material that is compatible with a vacuum environment. In 2006, the market for outsourced DLC coatings was estimated as about 30,000,000 € in the European Union.
Naturally occurring diamond is almost always found in the crystalline form with a purely cubic orientation of sp3 bonded carbon atoms. Sometimes there are lattice defects or inclusions of atoms of other elements that give color to the stone, but the lattice arrangement of the carbons remains cubic and bonding is purely sp3. The internal energy of the cubic polytype is slightly lower than that of the hexagonal form and growth rates from molten material in both natural and bulk synthetic diamond production methods are slow enough that the lattice structure has time to grow in the lowest energy (cubic) form that is possible for sp3 bonding of carbon atoms. In contrast, DLC is typically produced by processes in which high energy precursive carbons (e.g. in plasmas, in filtered cathodic arc deposition, in sputter deposition and in ion beam deposition) are rapidly cooled or quenched on relatively cold surfaces. In those cases cubic and hexagonal lattices can be randomly intermixed, layer by atomic layer, because there is no time available for one of the crystalline geometries to grow at the expense of the other before the atoms are "frozen" in place in the material. Amorphous DLC coatings can result that have no long-range crystalline order. Without long range order there are no brittle fracture planes, so such coatings are flexible and conformal to the underlying shape being coated, while still being as hard as diamond. In fact this property has been exploited to study atom-by-atom wear at the nanoscale in DLC.
SEM image of a gold-coated replica of a ta-C "diamond-like" coating. Structural elements are not crystallites but are nodules of sp3-bonded carbon atoms where lattice geometries randomly alternate between the cubic and hexagonal polytypes of diamond. The grains are so small that the surface appears mirror smooth to the eye.
There are several methods for producing DLC, but all depend upon the fact that in carbon the sp3 bond length is significantly less than the length of the sp2 bond. So the application of pressure, impact, catalysis, or some combination of these at the atomic scale can force sp2 bonded carbon atoms closer together into sp3 bonds. This must be done vigorously enough that the atoms cannot simply spring back apart into separations characteristic of sp2 bonds. Usually techniques either combine such a compression with a push of the new cluster of sp3 bonded carbon deeper into the coating so that there is no room for expansion back to separations needed for sp2 bonding; or the new cluster is buried by the arrival of new carbon destined for the next cycle of impacts. It is reasonable to envision the process as a "hail" of projectiles that produce localized, faster, nanoscale versions of the classic combinations of heat and pressure that produce natural and synthetic diamond. Because they occur independently at many places across the surface of a growing film or coating, they tend to produce an analog of a cobblestone street with the cobbles being nodules or clusters of sp3 bonded carbon. Depending upon the particular "recipe" being used, there are cycles of deposition of carbon and impact or continuous proportions of new carbon arriving and projectiles conveying the impacts needed to force the formation of the sp3 bonds. As a result, ta-C may have the structure of a cobblestone street, or the nodules may "melt together" to make something more like a sponge or the cobbles may be so small as to be nearly invisible to imaging. A classic "medium" morphology for a ta-C film is shown in the figure.
As implied by the name, diamond-like carbon (DLC), the value of such coatings accrues from their abilities to provide some of the properties of diamond to surfaces of almost any material. The primary desirable qualities are hardness, wear resistance, and slickness (DLC film friction coefficient against polished steel ranges from 0.05-0.20).
However, which properties are added to a surface and to what degree depends upon which of the 7 forms are applied, and further upon the amounts and types of diluents added to reduce the cost of production. In 2006 the Association of German Engineers, VDI, the largest engineering association in Western Europe issued an authoritative report VDI2840 in order to clarify the existing multiplicity of confusing terms and trade names. It provides a unique classification and nomenclature for diamond-like-carbon (DLC) and diamond films. It succeeded in reporting all information necessary to identify and to compare different DLC carbon films which are offered on the market. Quoting from that document:
These [sp3] bonds can occur not only with crystals - in other words, in solids with long-range order - but also in amorphous solids where the atoms are in a random arrangement. In this case there will be bonding only between a few individual atoms and not in a long-range order extending over a large number of atoms. The bond types have a considerable influence on the material properties of amorphous carbon films. If the sp2 type is predominant the film will be softer, if the sp3 type is predominant the film will be harder.
A secondary determinant of quality was found to be the fractional content of hydrogen. Some of the production methods involve hydrogen or methane as a catalyst and a considerable percentage of hydrogen can remain in the finished DLC material. When it is recalled that the soft plastic, polyethylene is made from carbon that is bonded purely by the diamond-like sp3 bonds, but also includes chemically bonded hydrogen, it is not surprising to learn that fractions of hydrogen remaining in DLC films degrade them almost as much as do residues of sp2 bonded carbon. The VDI2840 report confirmed the utility of locating a particular DLC material onto a 2-dimensional map on which the X-axis described the fraction of hydrogen in the material and the Y-axis described the fraction of sp3 bonded carbon atoms. The highest quality of diamond-like properties was affirmed to be correlated with the proximity of the map point plotting the (X,Y) coordinates of a particular material to the upper left corner at (0,1), namely 0% hydrogen and 100% sp3 bonding. That "pure" DLC material is ta-C and others are approximations that are degraded by diluents such as hydrogen, sp2 bonded carbon, and metals. Valuable properties of materials that are ta-C, or nearly ta-C follow.
STM image of surfaces at the edge of a 1 μm thick layer of ta-C "diamond-like" coating on 304 stainless steel after various durations of tumbling in a slurry of 240 mesh SiC abrasive. The first 100 min shows a burnishing away from the coating of an overburden of soft carbons than had been deposited after the last cycle of impacts converted bonds to sp3. On the uncoated part of the sample, about 5 μm of steel were removed during subsequent tumbling while the coating completely protected the part of the sample it covered.
Within the "cobblestones", nodules, clusters, or "sponges" (the volumes in which local bonding is sp3) bond angles may be distorted from those found in either pure cubic or hexagonal lattices because of intermixing of the two. The result is internal (compressive) stress that can appear to add to the hardness measured for a sample of DLC. Hardness is often measured by nanoindentation methods in which a finely pointed stylus of natural diamond is forced into the surface of a specimen. If the sample is so thin that there is only a single layer of nodules, then the stylus may enter the DLC layer between the hard cobblestones and push them apart without sensing the hardness of the sp3 bonded volumes. Measurements would be low. Conversely, if the probing stylus enters a film thick enough to have several layers of nodules so it cannot be spread laterally, or if it enters on top of a cobblestone in a single layer, then it will measure not only the real hardness of the diamond bonding, but an apparent hardness even greater because the internal compressive stress in those nodules would provide further resistance to penetration of the material by the stylus. Nanoindentation measurements have reported hardness as great as 50% more than values for natural crystalline diamond. Since the stylus is blunted in such cases or even broken, actual numbers for hardness that exceed that of natural diamond are meaningless. They only show that the hard parts of an optimal ta-C material will break natural diamond rather than the inverse. Nevertheless, from a practical viewpoint it does not matter how the resistance of a DLC material is developed, it can be harder than natural diamond in usage. One method of testing the coating hardness is by means of the Persoz pendulum.
 Bonding of DLC coatings
The same internal stress that benefits the hardness of DLC materials makes it difficult to bond such coatings to the substrates to be protected. The internal stresses try to "pop" the DLC coatings off of the underlying samples. This challenging downside of extreme hardness is answered in several ways, depending upon the particular "art" of the production process. The most simple is to exploit the natural chemical bonding that happens in cases in which incident carbon ions supply the material to be impacted into sp3 bonded carbon atoms and the impacting energies that are compressing carbon volumes condensed earlier. In this case the first carbon ions will impact the surface of the item to be coated. If that item is made of a carbide-forming substance such as Ti or Fe in steel a layer of carbide will be formed that is later bonded to the DLC grown on top of it. Other methods of bonding include such strategies as depositing intermediate layers that have atomic spacings that grade from those of the substrate to those characteristic of sp3 bonded carbon. In 2006 there were as many successful recipes for bonding DLC coatings as there were sources of DLC.
DLC coatings are often used to prevent wear due to its excellent tribological properties. DLC is very resistant to abrasive and adhesive wear making it suitable for use in applications that experience extreme contact pressure, both in rolling and sliding contact. DLC is often used to prevent wear on razor blades and metal cutting tools, including lathe inserts and milling cutters. DLC is used in bearings, cams, cam followers, and shafts in the automobile industry. The coatings reduce wear during the 'break-in' period, where drive train components may be starved for lubrication.
DLCs may also be used in chameleon coatings that are designed to prevent wear during launch, orbit, and re-entry of land launched space vehicles. DLC provides lubricity at ambient atmosphere and at vacuum, unlike graphite which requires moisture to be lubricious.
Despite the favorable tribological properties of DLC it must be used with caution on ferrous metals. If it is used at higher temperatures, the substrate or counter face may carburize, which could lead to loss of function due to a change in hardness. This phenomenon prevents the use of DLC coated machine tool on steel.
If a DLC material is close enough to ta-C on plots of bonding ratios and hydrogen content it can be an insulator with a high value of resistivity. Perhaps more interesting is that if prepared in the "medium" cobblestone version such as shown in the above figure, electricity is passed through it by a mechanism of hopping conductivity. In this type of conduction of electricity the electrons move by quantum mechanical tunneling between pockets of conductive material isolated in an insulator. The result is that such a process makes the material something like a semiconductor. Further research on electrical properties is needed to explicate such conductivity in ta-C in order to determine its practical value. However, a different electrical property of emissivity has been shown to occur at unique levels for ta-C. Such high values allow for electrons to be emitted from ta-C coated electrodes into vacuum or into other solids with application of modest levels of applied voltage. This has supported important advances in medical technology.
Applications of DLC typically utilize the ability of the material to reduce abrasive wear. Tooling components, such as endmills, drill bits, dies and molds often use DLC in this manner. DLC is also used in the engines of modern supersport motorcycles, Formula 1 racecars, NASCAR vehicles, and as a coating on hard-disk platters and hard-disk read heads to protect against head crashes. Virtually all of the multi-bladed razors used for wet shaving have the edges coated with hydrogen-free DLC to reduce friction, preventing abrasion of sensitive skin. Some forms have been certified in the EU for food service and find extensive uses in the high-speed actions involved in processing novelty foods such as "chips" and in guiding material flows in packaging foodstuffs with plastic wraps. DLC coats the cutting edges of tools for the high-speed, dry shaping of difficult exposed surfaces of wood and aluminum, for example on automobile dashboards.
The implantable human heart pump can be considered the ultimate biomedical application where DLC coating is used on blood contacting surfaces of the key components of the device.
Other medical applications such as Percutaneous coronary intervention employing brachytherapy find additional benefits from the unique electrical properties of DLC. At low voltages and low temperatures electrodes coated with DLC can emit enough electrons to be arranged into disposable, micro-X-ray tubes as small as the radioactive seeds that are introduced into arteries or tumors in conventional brachytherapy. The same dose of prescribed radiation can be applied from the inside, out with the additional possibility to switch on and off the radiation in the prescribed pattern for the X-rays being used.
 Environmental effects of durable products
Peer-reviewed research published in scholarly journals has established that the increases in lifetimes of articles coated with DLC that wear out because of abrasion can be described by the formula f = (g)µ, where g is a number that characterizes the type of DLC, the type of abrasion, the substrate material and μ is the thickness of the DLC coating in μm. For "low-impact" abrasion (pistons in cylinders, impellers in pumps for sandy liquids, etc.), g for pure ta-C on 304 stainless steel is 66. This means that one-μm thickness (that is ~5% of the thickness of a human hair-end) would increase service lifetime for the article it coated from a week to over a year and two-μm thickness would increase it from a week to 85 years. These are measured values; though in the case of the 2 μm coating the lifetime was extrapolated from the last time the sample was evaluated until the testing apparatus itself wore out.
There are environmental arguments that a sustainable economy ought to encourage articles not engineered to lower performance or to fail prematurely. This in turn will reduce the need to support greater production of units and their frequent replacement, which might provide an economic disincentive to manufacturers of such devices.
Currently there are about 100 outsource vendors of DLC coatings that are loaded with amounts of graphite and hydrogen and so give much lower g-numbers than 66 on the same substrates.
歡迎來到Bewise Inc.的世界，首先恭喜您來到這接受新的資訊讓產業更有競爭力，我們是提供專業刀具製造商，應對客戶高品質的刀具需求，我們可以協助客戶滿足您對產業的不同要求，我們有能力達到非常卓越的客戶需求品質，這是現有相關技術無法比擬的，我們成功的滿足了各行各業的要求，包括：精密HSS DIN切削刀具、協助客戶設計刀具流程、DIN or JIS 鎢鋼切削刀具設計、NAS986 NAS965 NAS897 NAS937orNAS907 航太切削刀具,NAS航太刀具設計、超高硬度的切削刀具、醫療配件刀具設計、複合式再研磨機、PCD地板專用企口鑽石組合刀具、粉末造粒成型機、主機版專用頂級電桿、PCBN刀具、PCD刀具、單晶刀具、PCD V-Cut刀、捨棄式圓鋸片組、粉末成型機、航空機械鉸刀、主機版專用頂級電感、’汽車業刀具設計、電子產業鑽石刀具、木工產業鑽石刀具、銑刀與切斷複合再研磨機、銑刀與鑽頭複合再研磨機、銑刀與螺絲攻複合再研磨機等等。我們的產品涵蓋了從民生刀具到工業級的刀具設計；從微細刀具到大型刀具；從小型生產到大型量產；全自動整合；我們的技術可提供您連續生產的效能，我們整體的服務及卓越的技術，恭迎您親自體驗！！
BW Bewise Inc. Willy Chen firstname.lastname@example.org email@example.com www.tool-tool.com skype:willy_chen_bw Head &Administration Office No.13,Shiang Shang 2nd St., West Chiu Taichung,Taiwan 40356 http://www.tool-tool.com/ / FAX:+886 4 2471 4839 N.Branch 5F,No.460,Fu Shin North Rd.,Taipei,Taiwan S.Branch No.24,Sec.1,Chia Pu East Rd.,Taipao City,Chiayi Hsien,Taiwan
Welcome to BW tool world! We are an experienced tool maker specialized in cutting tools. We focus on what you need and endeavor to research the best cutter to satisfy users’ demand. Our customers involve wide range of industries, like mold & die, aerospace, electronic, machinery, etc. We are professional expert in cutting field. We would like to solve every problem from you. Please feel free to contact us, its our pleasure to serve for you. BW product including: cutting tool、aerospace tool .HSS DIN Cutting tool、Carbide end mills、Carbide cutting tool、NAS Cutting tool、NAS986 NAS965 NAS897 NAS937orNAS907 Cutting Tools,Carbide end mill、disc milling cutter,Aerospace cutting tool、hss drill’Фрезеры’Carbide drill、High speed steel、Compound Sharpener’Milling cutter、INDUCTORS FOR PCD’CVDD(Chemical Vapor Deposition Diamond )’PCBN (Polycrystalline Cubic Boron Nitride) ’Core drill、Tapered end mills、CVD Diamond Tools Inserts’PCD Edge-Beveling Cutter(Golden Finger’PCD V-Cutter’PCD Wood tools’PCD Cutting tools’PCD Circular Saw Blade’PVDD End Mills’diamond tool. INDUCTORS FOR PCD . POWDER FORMING MACHINE ‘Single Crystal Diamond ‘Metric end mills、Miniature end mills、Специальные режущие инструменты ‘Пустотелое сверло ‘Pilot reamer、Fraises’Fresas con mango’ PCD (Polycrystalline diamond) ‘Frese’POWDER FORMING MACHINE’Electronics cutter、Step drill、Metal cutting saw、Double margin drill、Gun barrel、Angle milling cutter、Carbide burrs、Carbide tipped cutter、Chamfering tool、IC card engraving cutter、Side cutter、Staple Cutter’PCD diamond cutter specialized in grooving floors’V-Cut PCD Circular Diamond Tipped Saw Blade with Indexable Insert’ PCD Diamond Tool’ Saw Blade with Indexable Insert’NAS tool、DIN or JIS tool、Special tool、Metal slitting saws、Shell end mills、Side and face milling cutters、Side chip clearance saws、Long end mills’end mill grinder’drill grinder’sharpener、Stub roughing end mills、Dovetail milling cutters、Carbide slot drills、Carbide torus cutters、Angel carbide end mills、Carbide torus cutters、Carbide ball-nosed slot drills、Mould cutter、Tool manufacturer.
Bewise Inc. www.tool-tool.com
（２）Carbide Cutting tools設計
Bewise Inc. talaşlı imalat sanayinde en fazla kullanılan ve üç eksende (x,y,z) talaş kaldırabilen freze takımlarından olan Parmak Freze imalatçısıdır. Çok geniş ürün yelpazesine sahip olan firmanın başlıca ürünlerini Karbür Parmak Frezeler, Kalıpçı Frezeleri, Kaba Talaş Frezeleri, Konik Alın Frezeler, Köşe Radyüs Frezeler, İki Ağızlı Kısa ve Uzun Küresel Frezeler, İç Bükey Frezeler vb. şeklinde sıralayabiliriz.
BW специализируется в научных исследованиях и разработках, и снабжаем самым высокотехнологичным карбидовым материалом для поставки режущих / фрезеровочных инструментов для почвы, воздушного пространства и электронной индустрии. В нашу основную продукцию входит твердый карбид / быстрорежущая сталь, а также двигатели, микроэлектрические дрели, IC картонорезальные машины, фрезы для гравирования, режущие пилы, фрезеры-расширители, фрезеры-расширители с резцом, дрели, резаки форм для шлицевого вала / звездочки роликовой цепи, и специальные нано инструменты. Пожалуйста, посетите сайт www.tool-tool.com для получения большей информации.
BW is specialized in R&D and sourcing the most advanced carbide material with high-tech coating to supply cutting / milling tool for mould & die, aero space and electronic industry. Our main products include solid carbide / HSS end mills, micro electronic drill, IC card cutter, engraving cutter, shell end mills, cutting saw, reamer, thread reamer, leading drill, involute gear cutter for spur wheel, rack and worm milling cutter, thread milling cutter, form cutters for spline shaft/roller chain sprocket, and special tool, with nano grade. Please visit our web www.tool-tool.com for more info.